1 CONTENTS 1. Injection Molding Machine 1.1 Injection Unit 1.2 Clamping Unit 1.3 Multi-program Control 1.4 Defective Molding, Causes and Remedies 2. Molding Operation 2.1 Preliminary drying of materials Dryer 2.2 Molding Conditions 2.3 Other cautions 2.4 Product Quality Control 2.5 Material replacement Interruption of Operation Cleaning by Dismantling 3. Product Design and Mold Design 3.1 Product Design 3.2 Mold Design 4. Mold Shrinkage and Dimensional Accuracy 5. CAE 6. Hot Runner Molding 7. Reuse of Iupilon / NOVAREX 8. Annealing Treatment of Iupilon / NOVAREX 8.1 Annealing Treatment 8.2 Annealing Effect of using both hot air / far infrared radiation heating system International System of Units (SI units)
2 1. Injection molding machine As for the injection molding machine, several types such as plunger type, plunger preplasticating type, screw preplasticating type and in-line screw type, etc. have been developed so far, but presently the in-line screw type injection molding machine as shown in Figure has become the main type. moving plate heated cylinder fixed plate band heater hopper injection cylinder mold screw Figure Theory of the in-line screw type injection molding machine The injection molding machine consists of the injection unit and the clamping unit, and their features are described below. 1 1 Injection unit 1)Injection capacity The proper injection capacity is found from the relationship of the molding machine capacity for the weight of 1 shot as shown in Figure It is necessary to select the molding machine that satisfies the capacity of the shaded area. This figure is the summary of the actual molding results in the past, but basically, it is based on the following idea. injection molding machine capacity good molding area excessive capacity area 1 shot weight (g) insufficient capacity area Fig Selection of molding machine from the injection capacity
3 At the side where the capacity is small, plasticizing time and injection time become long, and it is used at the narrow capacity of the molding machine. That is, the filling shortage is caused due to the extension of molding cycle and slow filling rate. On the other hand, at the side where the capacity is large, dwell time of the resin inside the cylinder becomes long, and the resin thermally decomposes. The capacity range in the figure is indicated rather widely, but when it is easy to be thermally decomposed with materials containing lots of pigments and additives, it is better to conduct the molding at shot weight of 70~80% of the injection capacity. 2 Barrel Generally, using the material (for example, nitride steel etc.) for the molding of Iupilon / NOVAREX is good. However, concerning the molding of glass fiber reinforced grade (Iupilon GS etc.) and optical grade (Iupilon H-400 etc.), it is good to consider the following for the barrel material. As for glass fiber reinforced PC, it is good to use the bimetal (double-structure cylinder covered the inside with another metal and centrifugal casting) to prevent the barrel abrasion. For example, the H alloy (Hitachi Metals Ltd.), N alloy (Japan Steel Works Ltd.), K alloy (Kobe Steel Ltd.) etc. are well known. Figure indicates the abrasion data when molding glass fiber (30%) PC in case of using the H alloy barrel. The abrasion of the metering section vicinity where the feed section and the backflow prevention ring contact with is improved 1). In addition, the bimetal cylinder such as H alloy is also effective in suppressing the generation of the burn of Iupilon / NOVAREX although the burn mark and black specks due to thermal decomposition become problems in the transparent use. 1) Hitachi Metals Ltd. H alloy catalogue cylinder hopper variation of inner diameter molding resin nitrided steel cylinder after 6-month use (disposed after measuring) H-503 cylinder after 1 and a half year use (prolonged use) type characteri stic alloy hardness system longitudinal heat expansion coefficient ( ) anti-wear, anti-corrosion distance from the cylinder tip (mm) Fig Barrel material and abrasion data when using GF (30%) PC
4 3) Screw The 3-stage type screw of the single flight is usually used. The screw design consists of the basic design based on the premises of smooth conveyance of pellet, plasticization for melting, dearation and compression, and measurement with a little unevenness. Supply (feed section): Stroke is designed long for conveying and melting the pellet, and increasing plasticization quantity. Compression (compression section): Return the air and water involved in the feed section to the hopper side and deaerate. In addition, a sufficiently melting mechanism is required. Because PC is a high viscosity material, the rapid compression type is unsuitable and moderating compression type with gradually increasing outside diameter is recommended. Measurement (metering section): In order to suppress the measurement unevenness, the measurement stroke is designed long, 4D ~ 5D or more. The screw design of PC is indicated in Fig ) screw head backflow prevention ring sealing pitch outer diameter head metering section compression section feed section Notes: in ( ) shows an example of total length L Basic shape of screw stroke metering zone compression zone feed zone screw length Screw depth Screw diameter Feed section Metering section Compression ratio mm mm mm Max 14 0 Max 5 6 Max Screw pitch H=1.0D Screw diameter more than 80mm H=0.9D Screw diameter less than 80mm Fig Design of screw for PC ) Jonathan M. Newcome:SPE Tech Pap Reg Tech Conf. PIONEER VALLEY SEC ( 77 june 8/9) 45 78
5 In the same figure, L/D is 20, the ratio of Feed (F) / Compression (C) / Metering (M) is divided into 60/20/20, pitch H is almost equal to screw diameter D, and compression ratio C.R. of the screw is 2.0:1~2.5:1. The screw that its surface is covered with thick film hard Cr coating is good. When the glass fiber reinforced material is used, there is a problem of abrasion, but constantly preparing spare screw and regularly exchanging after recoating are recommended. The screw that processed nitriding treatment is hard to be worn due to its high hardness. On the other hand, for transparent product and colored product (except the black) avoiding the burn, because it is easy to cause the burn in PC molding, it had better use the screw that processed with (Ni+Cr), (Co+Cr), TiC treatment at the surface though it is a little expensive. Recently, the example which uses dulmage,, pin screw mounted at the screw head with the purpose to improve the melting and mixing and the dispersibility is observed with the precondition of not giving excessive shearing force to PC and the design without PC stagnation. 4 Backflow prevention valve, check ring The screw head is equipped with the backflow prevention valve to maintain the effective injection pressure by preventing a part of measured resin from backflow through the ditch of the screw at the time of injection. The structure of this valve is indicated in Fig It can be understood that it is easy for resin stagnation with this valve structure. Therefore, the design of the flow path without dead space by taking enough R so as not to provide the corner as much as possible is expected. In addition, as for high viscosity material such as PC, because torque is big, the fatigue failure occurs in the screw of small aperture when receiving the load by repeated rotation, the use of screw of wide aperture is recommended. Back flow ring type equipped with nail cross-section drawing Fig Design of Shut Off Valve
6 As for compound reinforced PC such as glass fiber reinforced material etc. the backflow prevention ring sometimes cracks when the load becomes large compared with the non-reinforced material. When molding without being aware of this, the uneven dimension and the deviation from tolerance in the molding of a precise part occur due to the unstable measurement. It is necessary to note that such a trouble easily occurs in case of overload and insufficient purge. 5 Nozzle A nozzle with the structure without PC stagnation is desirable as possible. Therefore, it is necessary to avoid using the needle shut off nozzle and torpedo nozzle due to resin stagnation. The open nozzle is the best for use. The open nozzle is easy to cause drooling, stringiness, and it is difficult to prevent them but using a long-extended nozzle and adjusting independently the temperature at two separate places of the tip and the bottom, are effective. 6 Heater Since PC is molded at high temperature, the heater with heat capacity can be heated to about 370 is used, and a band heater is usually used. When disassembling to clean the nozzle and cylinder head and when the heater is stuck with drooling resin, the heater is disconnected. It is necessary to note that it is easy to cause the burn when continuing molding without being aware of heater disconnection. 1 2 Clamping unit As for the molding of Iupilon / NOVAREX, either the hydraulic type or the toggle type is available. Since the average value of the mold internal pressure in the molding of Iupilon / NOVAREX is kg/cm2, the clamping force F can be calculated by the following equation. F(ton)=(0.35~0.50) S where S: projected area as indicated in Fig However, it is necessary to note that when the arrangement of molding is eccentric from the center of mold (center of die plate), the clamping force, which is higher than the above formula is required. clamping pressure of the molding machine (ton) projected area of the molded piece Fig Selection of molding machine from clamping pressure
7 1 3 Multistep program control The improvement of poor appearance of the moldings, the reduction of size unevenness between the molding shots, and the measures against sink marks, warpage and flash can be achieved by controlling the injection rate, holding pressure, screw rotation speed and back pressure with multistep program control at the time of injection. The effect of multistep program control in PC and its control system are indicated in Fig The outline is introduced below. 3) Table Effect of multistep control (in case of PC) Molding conditions Injection rate Effect Prevention of jetting mark at gate part, prevention of flow mark of sharp corner, prevention of core falling and prevention of flash Holding pressure Screw rotation speed Back pressure Reduction of molding stress and prevention of sink mark Stability of measurement Stability of measurement 3: Screw position detector 5: Injection rate detector 10: Screw rotation speed detector 7: Pressure detector 1: Servo valve 2: Servo valve 4: Program setting device 6: Injection rate controller 9: Holding pressure controller 8: Screw back pressure controller 11: Screw rotation speed controller input feedback Disturbance Comparison controller Setting value Controller Controlled object Control variable Detecting value Detector Fig Outline of multistep program control system
8 Control of the injection rate Since the poor appearance is resulted from the change of rate of the flow front, the measures can be done by controlling the injection rate. The relationship between the flow rate and the defective phenomena is summarized in Table It can be understood that the injection rate should be set to an appropriate range because there is a problem even if the flow rate is too fast or too slow. Table Flow rate and defective phenomena Defective phenomena results from too slow flow rate of resin Flow mark Transcription defect of mold surface Weld line Short shot Defective phenomena results from too fast flow rate of resin Jetting mark Gas burn Sink mark due to trouble of air purge Fig indicates an example of a measure to avoid the area of various defective phenomena by controlling the injection rate with multistep program control. It is understood that the setting range of the injection rate to have a product of good quality is narrow (shaded part) in case of general molding. gas burn jetting area to obtain good product when setting program of injection rate injection rate area to obtain good product when not setting program of injection rate weld line screw stroke Fig gate flow mark transcription defect of mold surface Defective area of injection rate Control of the holding pressure The defective phenomena such as sink marks, warpage and flash are related to the holding pressure. The measure against these phenomena becomes possible by controlling the holding pressure. The relationship between the defective phenomena such as sink marks, warpage and flash and the holding pressure is summarized in Table Figure indicates the pattern of the holding pressure program which was obtained to avoid the defective phenomenon area )Sumitomo Heavy Industries, Ltd. Plastic Machinery, lecture textbook of injection molding Molding B Course Practical Application
9 Table Holding pressure and defective phenomena Defective phenomena results from too low holding pressure Short shot Sink mark Underdimension Shrinkage strain Defective phenomena results from too high holding pressure Flash Overdimension Crack Mold release defect Residual stress warpage flash sink mark holding pressure holding pressure time Fig Holding pressure pattern to avoid defective area Control of screw back pressure and screw rotation speed The stability of measurement (plasticization) is related to screw back pressure and screw rotation speed. It is possible to improve the accuracy of uneven repeated measurement by controlling these factors. Fig indicates the result of comparing the effects of the multistep program control of screw back pressure and screw rotation speed about the measurement position or mold release resistance 4). From this figure, it is thought that the unevenness of the measurement position, mold release resistance was decreased by the multistep program control.
10 mold release resistance (kgf) shot number no program control measurin g position Sg (mm) shot number mold release resistance (kgf) shot number with program control measurin g position Sg (mm) shot number Fig Stabilization by the program control of plasticization process (Material:S-2000)
11 1 4 Defective Moldings, Causes, and Remedies Defects to be encountered in molding of Iupilon / NOVAREX are almost similar to those of other plastic materials. The defective causes and remedies of general grade and glass fiber reinforced grade are summarized in Tables and 1 4-2, respectively. The effect that the mold temperature of glass fiber reinforced grade has on the appearance is indicated in Fig Table shows the problems and remedies in an accurate molding. Table Defective causes and remedies of general grade
13 Table Defective causes and remedies of glass fiber reinforced grade
14 Fig Relation between the mold temperature and the appearance of glass fiber reinforced grade Color difference: the color difference with glass reinforced PC (black) was obtained by considering the non-reinforced PC (black) as a controlled material.
15 Table Defective causes and remedies in an accurate molding
16 A Measures regarding the materials B Measures regarding the molding machine, auxiliary equipment etc. C Measures regarding the product design, molding conditions etc. D Measures regarding the mold design
17 2. Molding operation 2 1 Preliminary drying of materials Dryer Since Iupilon / NOVAREX have an ester bond in the main chain, the hydrolysis occurs when heated with the moisture. As a result, the physical properties, particularly the molecular weight and the impact strength are reduced. Also, the preliminary drying before molding is necessary because the generation of silver streak and void at the appearance occur. The moisture content in the pellets should be assumed to be 0.015~0.020% at the preliminary drying of Iupilon / NOVAREX. The results of the molding at various moisture content are shown in Table These results indicate that the degradation of the impact strength in addition to the generation of defective appearance is very large. Therefore, it is important to use the dried pellets that the moisture content is lower than the above mentioned limit to have a good performance of Iupilon / NOVAREX. Table Effect of the moisture content at the time of injection molding S-2000(Molecular weight ) Moisture content Molecular Falling ball impact destruction rate weight of molded pieces Ductile failure Brittle failure Total destruction rate Appearance of molded pieces Good Good Good A few silver streak Silver streak, bubble (Note) Weight of falling ball impact test 2.13kg. The head makes the heavy bob of 10mmR fall from the height of 10 m The drying conditions of Iupilon / NOVAREX are indicated in Table Table Drying conditions of Iupilon / NOVAREX Drying conditions Temperature Time required Notes Many examples of use. Multi-tray hot air Pay attention to the ambient moisture circulation dryer hr or more Thickness less than 30mm is preferable. Many examples of use Pay attention to the ambient moisture Hopper dryer hr or more and short circuit pass When the input is small, the moisture distribution is bad. Dehumidifying It is often used for the molding of Hopper Dryer hr or more optical disk substrate and optical lens etc. In order to dry the pellets of Iupilon / NOVAREX until the moisture content is lower than the above mentioned limit it is necessary to note the kind of the dryer, its performance and environment ( temperature and moisture). Fig is the example which shows the dry curve by the difference of the environment with the multi-tray hot air circulation dryer. The dry efficiency is decreased under high temperature, high humidity and it requires long time until the moisture content is lower than the limit.
18 Also, Fig shows the results obtained by the hopper dryer in the same way. The dehumidification hopper dryer that is not affected by the environment and the dry efficiency is good. However, it is necessary to pay attention to the time degradation of the dehumidifier performance and consider the short pass phenomenon of the pellets when determining the drying capacity. capacity set temperature atmosphere 50kg feed water absorption percentage (%) limiting water absorption(0.02%) drying time (hr) Fig Multi-tray hot air circulation dryer capacity set temperature atmosphere 50kg feed water absorption percentage (%) limiting water absorption(0.02%) drying time (hr) Fig Drying conditions by the hopper dryer Prevention of moisture absorption in the hopper It is necessary to pay attention to the moisture re-absorption in the molding machine hopper in addition to the preliminary drying of the pellets as described in Section 2 1. Moreover, it is also necessary to consider preventing the moisture re-absorption by shortening the installation of the hopper dryer, hopper insulation and dwell time of the pellets as much as possible.
19 2 2 Molding conditions 1) Cylinder temperature The resin temperature is often higher than the setting temperature of the cylinder by C. It is good to measure the characteristic of the injection molding machine to use in advance. The general molding temperature of Iupilon / NOVAREX is in the range of 260~320 C, but it is better to set it as low as possible for deep colored products. As for the setting of the cylinder temperature, it is common to set the temperature gradient such that the hopper side is higher by C. When the rotation torque of the screw becomes overload by the high viscosity grade and so on, the temperature on the hopper side may be set high oppositely.. In addition, the selection of the molding temperature should be made in consideration of the molding cycle time, namely the dwell time of the resin in the cylinder. The molding machine with the injection capacity by corresponding to the weight of the molded pieces and molding conditions is selected, and the dwell time is shortened as much as possible to avoid the thermal degradation of the resin. It is necessary to note that the temperature of the nozzle has a slight affect on the cold flow of the molded pieces and the leakage of the resin (drooling). 2) Injection pressure, holding pressure The injection pressure and holding pressure are set as low as possible if the sink marks and voids do not occur in the molded pieces. However, in case of the resin with high melt viscosity such as Iupilon / NOVAREX, the inside of the mold can not be filled from the pressure loss with the flow process of the resin if the pressure is not raised to some degree. As soon as the cavity is filled, the injection pressure is reduced to the level that does not cause sink marks. In addition, the pressure is raised to reduce the mold shrinkage of the resin, but from the point of strain and mold release characteristic which remain in the molded pieces, the pressure should be set as low as possible. 3) Injection rate As indicated in Fig , since the flow length increases when the injection rate increases, the fast filling is carried out for thin-walled molded pieces. However, when the fast filling is carried out, defects such as flow marks and flash are produced. Since the recent injection molding machine is equipped with the multistep control of the injection rate (program injection), both the filling and appearance can be controlled by changing the rate according to the shape and gate of molded pieces. The basic rate program is as follows. (a) Make high speed at the passage of the sprue and runner part. (b) Make low speed at the initial filling of the gate part and product part, and at the time of filling completion. (c) Make low speed when passing over the thin type core and pin part.
20 flow length exclusive of gate (mm) Iupilon injection rate Fig Injection rate vs Flow length 4) Rotation speed of screw and Back pressure It is necessary to increase the rotation speed of screw to shorten the plasticizing time but it becomes the cause of air entry, generation of the resin burning, bubble and silver streaks resulting from the deaeration insufficiency, and easy to cause the thermal degradation by adiabatic exothermic heat. The back pressure is about 5-10 % of the injection pressure to improve the deaeration effect on the hopper side. Since the back pressure has an affect on the leakage (drooling) of the resin from the nozzle, the consideration of setting temperature is also necessary. 5) Mold temperature The mold temperature is one of the important conditions in the molding of Iupilon / NOVAREX. When the mold temperature is too low, the filling becomes bad, and in addition to the defective appearance such as flow marks etc., the molding strain is easy to be generated. On the other hand, when the mold temperature is too high, the resin is easy to stick to the mold surface and defect of the mold release and deformation of the molded pieces after the mold release easily occur. The standard mold temperature is 70~120.
21 2 3 Other cautions The mold release agent is selected and used according to the usage of the molded piece and the presence of the secondary processing. The mold release agents of silicone derivatives are usually used, but in case of printing and hot stamp, painting etc.as secondary processing, and cloudiness in the vicinity of the gate just after the application, it is better to use the paintable type or unused. 2) It is necessary to pay attention to the shape, removing fat and washing in case of inserts (refer to Iupilon Technology Report, PCR304 for detail). Sharp corners should be avoided in inserts (Fig ). Fig Shape of a blind insert The thickness of the molded pieces around the insert is necessary to be 0.5 times the diameter of the insert even in the worst case because it has an affect on the strain around the insert. In addition, if the insert is a metal in large size, preheating is necessary. In case a large number of inserts are to be used, the dwell time of the resin in the cylinder is prolonged because it takes long time for the mold installation and as a result, the thermal degradation of the resin may take place. Carrying out the insert after the molding is better. 2 4 Product quality control Strictly speaking, the molding operation is not over when the material feeding is converted into molded pieces, but it is necessary to check whether the pieces exhibit enough strength in actual use. From this point of view, it is very important to select proper molding conditions. The evaluation is not easy although molding conditions are modified and selected while judging their performance in actual use. The requested characteristics of the molded pieces are based on the basis of the customer s specification, and it is impossible to conduct everything in the molding process. The management is thoroughly executed in the early stage when producing a new molded piece, and it is necessary to focus on the point and to conduct day-by-day management afterwards. The item that should be managed in the molding process is to prevent the reduction of strength of molded piece due to 1. the degradation and decomposition of the resin, 2. molding strain. This is explained as follows. 1) Degradation, Decomposition of the resin Measurement of the molecular weight is used as a means to examine the degradation and decomposition of Iupilon / NOVAREX. It is necessary to note that the measurement of the molecular weight is difficult in a special grade, and can not be judged only by it in some cases. Since the measurement of the molecular weight is time consuming, it is better to conduct it at the stage of selecting the molding conditions at the beginning and to keep the correlation with other simple test method, and then manage it For example, it is also good to bend a sprue and a runner and examine the condition of breakage or conduct an impact test sensitive to the reduction in the molecular weight due to the decomposition of the resin (falling ball impact test etc. to add the impact in the molded piece with the hammer).
22 2 Molding strain A method often used for determination of the molding strain (residual stress) is to immerse Iupilon / NOVAREX in specific solvents to observe the presence of cracks generated. As for Iupilon / NOVAREX general grade, it is inspected by using the combined solvent of MIBK (methyl isobutyl ketone) and methanol. This method is suitable for stress detection by the following reasons. (a) In case of crack generation, a relatively big crack is generated and is easy to determine. (b) The detected stress can be changed by changing the mixed composition. Table is summarized based on current practical results. However, because the detection method of residual stress by solvent is a method of large unevenness actually, the result should be considered as a rough standard and an evaluation standard in correspondence with practical test must be decided. Also, the correspondent mixed composition of the conventional carbon tertrachloride / butanol system was described Table Mixed composition volume ratio Detected stress MPa MIBK Methanol CCl4 Butanol kg cm MIBK 50 CCl Evaluation Too severe for checking stress of normal molded piece Suitable for searching molding conditions for stress reduction and annealing conditions Molded piece is suitable for stress check in a simple substance. Suitable for the check of assembly articles and insert articles loaded by joint stress and external force. When the crack is generated at this level, there is a possibility that the crack is generated in actual use, too. After the sample is immersed in the mixed solvent of MIBK (methyl isobutyl ketone) and methanol for one minute, take it out, conduct water washing and observe the crack.
23 2 5 Material replacement, Interruption of Operation, and Cleaning by Dismantling 1) Material replacement Polyamide, polyacetal etc. should not be replaced directly with Iupilon / NOVAREX and the reverse is also similar. It is because these resin materials decompose when replacing directly to the molding temperature range of Iupilon / NOVAREX, and also promote the decomposition of Iupilon / NOVAREX. In such a case, polyethylene and polystyrene must be used between the two. However, it is necessary to note the case when a transparent resin such as polystyrene is mixed with Iupilon / NOVAREX because the end point of the replacement can not be clearly discernible. Recently, to make the replacement of color, material easy, various replacement materials (cylinder washing material) are available in the market. A proper replacement material can be selected according to the molding temperature range of the material before replacement, the material of the replacement purpose. Interruption of Operation, and Cleaning by Dismantling The resin is gradually decomposed and formed a carbonized layer on the internal surface of the heating cylinder and around the backflow prevention ring of the screw over a long period of operation. This carbonized layer does not peel off during the normal molding operation. However, when the temperature of the heating cylinder goes down during interruption of the operation, the carbonized layer peels off due to shrinkage, contaminates the molded pieces and becomes black specks when the molding operation is resumed. Therefore, it is better to keep the heating cylinder at during interruption of the operation for a short time. When the operation is stopped for a long time, it is good to replace Iupilon / NOVAREX with other resins of lower molding temperature range and lower the temperature. Polyethylene and polystyrene are good as replacing resins. Since the carbonized layer on the internal surface of the heating cylinder and around the backflow prevention ring of the screw gradually becomes thick and begins to contaminate the molded pieces when the decomposition progresses, the heating cylinder and the screw should be dismantled and cleaned regularly. Especially, since the contamination of foreign matters, black specks are not good for transparent molded pieces, it is necessary to dismantle and clean once every several months. When various resins are molded with the same molding machine, it is necessary to dismantle and clean the cylinder and the screw regularly. The dismantling procedure is done by replacing with polyethylene and polystyrene after the resin in the cylinder is emptied as much as possible. After dismantling, remove the remaining melted resin quickly, and then remove the carbonized layer with the spatula and brush made of cupper or burn with the burner. If Iupilon / NOVAREX remains and it is impossible to take it out, an effective method is to wash with a solvent such as methylene chloride etc. In this case, pay attention to the work environment (ventilation, fire).
24 3. Product design and Mold design 3 1 Product design When using Iupilon / NOVAREX, the contents shown in Table are considered as problems in practical use. As shown in Table 3 1-2, it is necessary to investigate and examine sufficiently so as not to cause these problems. In addition, the calculating formula shown in Table is useful for the standard of lightening, decision of the product thickness, and the selection of molding machine, etc. Classification Contents Crack and deterioration of impact strength due to degradation at the time of molding Breaking due to excessive load stress Strength Dimension Appearance Deterioration of strength due to concentration of stress Crack of insert and screw tightening part Solvent crack due to oil, plasticizer etc. Deterioration due to hot water and alkali. Defect of dimensional due to error of estimation of mold shrinkage factor Deformation due to excessive stress and warpage at the time of molding. Deformation due to creep deformation and thermal expansion. Silver streaks sink marks flow marks specks weld line hue non-uniform Uneven brightness of embossing uneven brightness of weld part, floating of glass fiber Table Points to be checked at the time of PC molding Classificatio Items n Reason of PC molding commercialization schedule weight and material, production General quantity, price in the past Required Lifetime, strength, dimension accuracy, rigidity, flammability, electrical property performance Temperature, chemical atmosphere (oil, solvent, hot water), kind of contacted substance Use (PVC, packing), outdoor use or not. environment Tightening Inserting, screw tightening, bonding, caulking. method Appearance Hue, existence of embossing existence of coating
25 Points to be checked at the time of PC molding Next, in order to maximize the good performance of Iupilon / NOVAREX, it is necessary to pay sufficient attention to the shape design. The key points are as follows: (1) The thickness is uniform and no sudden change of the thickness. (2) An acute angle is absent. (3) Provide a proper taper. (4) Undercuts are absent. As for the main items, the standard and cautions in the molding are described in order as follows. 1) Thickness The thickness of the molded piece should be decided in consideration of the required performance of the product and moldability of the material. The relationship between the thickness and the flow length for Iupilon / NOVAREX is shown in Fig. In case where the thickness is extremely thin, defect of unfilling, when it is extremely thick, defects such as sink marks, bubbles, deformation etc. and impact strength deterioration occur (thickness 5 mm or more). In addition, the sudden change of the thickness obstructs the flow of resin causes flow marks, notch effect at the corner, and weakening of strength. Examples of the design to have the uniform thickness are shown in Fig. The distribution standard of thickness is shown in Fig
26 flow length exclusive of gate (mm) I: Region where ordinary molding is possible II: Region where high temperature and pressure are required thickness (mm) Fig The relationship between the wall thickness and the flow length for Iupilon / NOVAREX bad good bad good bad bad bad bad good good good good flow direction Fig bad Distribution of the thickness flow direction OK flow direction good Fig Change of the thickness
27 2) Corner R The range of 0.5~1.0mmR is suitable for the corner. Since an excessive stress occurs at the corner of the molded piece due to the concentration of stress, be sure to provide R at the corner. The relationship between the notch R and the impact value for Iupilon / NOVAREX is shown in Fig The brittle fracture is shown when the notch R is below 0.1R. The relationship between the corner R and the stress concentration factor is shown in Fig When the corner R is small, the stress concentration factor becomes large, and as a result, it is easy to cause cracks, residue stress becomes large and defects such as flow marks easily occur. On the other hand, if the corner R is too large, defects such as sink marks, bubbles, and deformation etc. occur. Therefore, the ratio of the corner R and the thickness (R/T, R'/T), as shown in Fig. must be noted for the design of the corner. Thickness 1/8 inch, cutting notch pressure concentration coefficient corner radius R thickness ductile failure Izod impact value (J/m) brittle failure Fig The relationship between the corner R and stress concentration factor Fig The relationship between the notch R and Fig Design of the corner R impact value for 3) Weld Iupilon line / NOVAREX In addition to the deterioration of strength, various defective phenomena at the weld part are observed as shown in Table The reinforcement measures at the weld part such as the gate type, gate position, rib reinforcement etc. as shown in Fig are effective. Table Defective phenomena observed at the weld part Phenomena Practical failure Notes Deterioration of strength Deterioration of tensile elongation and impact strength Mainly observed in glass fiber reinforced grade, polymer alloy grade Generation of Generate in the vicinity crack of insert, screw boss Defect of Irregular color, Uneven Mainly observed in deep colored-substance
28 appearance brightness of embossing and polymer alloy grade Defect of dimension Sink marks, roundness defect Many defects in glass fiber reinforced grade A. Take the gate in the direction where the deposited area of the weld becomes large weld line gate B. Reinforce the rib in the vicinity of the generated hole of the weld line. C. Select the position of gate as the weld line does not generate in the vicinity of the insert metal fitting Gate A (good) Weld line does not generate Gate B (bad) Weld line generates Fig Examples of design of the weld part 4) Shape of Rib It is good to think that the design of a rib is almost the same as other plastic materials. Namely, the measure to prevent the generation of sink marks on the rib opposite side, and the notch effect at the corner part etc. is necessary. The design standard of a rib is shown in Fig Do not forget to provide R above 0.5~1.0mmR at the base corner of the rib. Fig Design of a rib
29 5 Tapering In general, the standard of a taper is in the range of 1/100~1/50 (0.5~1.0 ). An example of the molded piece with a deep rib is shown in Fig slope slope slope Fig Example of taper 6) Undercut There is no problem when missing an undercut by using the side core, but when pulling out an undercut by force with a normal mold, it is difficult to take a deep undercut because of the high mechanical strength and elasticity modulus of Iupilon / NOVAREX. The mold release possible undercut in case of a cylindrical piece as shown in Fig. can be calculated by the following equation. L Sprue Molded piece Undercut Core Stripper plate Fig Peripheral undercut R on the cylindrical piece
30 The design standard of a boss is shown in Fig Fig Boss 8) Hole It is necessary to note that when the edge and the hole of the molded piece come close, it results in the weakening of mechanical strength. Refer to Fig for the design of the hole. A 2D B D Fig Hole However, the load is generated only in an instant at the time of assembly, and it becomes 0 afterwards. Take a proper R. Fig Snap fit Fig Press fit Metal insert Hot compression B A B A Cold compression * % B Resin insert (PC-PC) B A Cold compression * % B As for the resin with elasticity modulus lower than that of PC, it is good to add to the above.
31 3 2 Mold Design Since the productivity and quality of the molded piece are greatly influenced by the mold design, the mold design is extremely important issue. The basic concept of the mold design is as follows. (1) The filling of the resin can be easily done, (2) The mold release can be easily done. (3) Pay attention to the control of the mold temperature. (reduction of non-uniform dimension including the shape, appearance of the product and stabilization of quality) Each item of the mold design is explained in order as follows. 1 S p r u e Basically, the sprue should be shaped as thin and short as possible. The points which should be noted are the mold release characteristic and air bubble of the base. As for the mold release, the draft should be as shown in Fig As for the air bubble of the base, it is important to design the diameter of the base to the suitable thickness. When the air bubble occurs at the base in the direct sprue, it results in the cutting of the sprue, defect of the product at the time of mold releasing. The diameter for not causing the air bubble at the base is as follows: The diameter of the sprue base 3 5mm Sprue cutting position Fig Shapes of the nozzle and the sprue bushing The pressure loss of the sprue part can be calculated by the following equation. It is preferable to reduce the pressure loss as much as possible. pressure loss of the sprue part
32 2 R u n n e r Fig Cross sections of runners The following empirical relationship between the length and thickness of the runner is the common practice. In the case of a multi-cavity mold, it is preferable to balance the runner length to each cavity, and all the cavities should be filled simultaneously as shown in Fig and Also, when it is difficult to balance the runner length, it is preferable to balance the gate for simultaneous filling as shown in Fig.
33 Fig Circular arrangement of cavities Fig Parallel arrangement of cavities Fig Linear arrangement of cavities
34 The pressure loss of the runner part can be calculated by the following equation. It is preferable to reduce the pressure loss as much as possible. pressure loss of the runner part viscosity of the resin olume flow of the resin runner length h y d r a u l i c d e p t h o f t h e r u n n e r p a r t S cross section area of the runner part l circumferential length cut of the runner part 3 G a t e The direct gate, side gate, pinpoint gate, submarine gate and tab gate can be applicable to the gate shapes. The side gate and pinpoint gate are commonly used as the gate shapes of Iupilon / NOVAREX molded piece. When the thickness of the side gate is thin, defective appearance such as unfilling, jetting marks occurs. From the market results, it is often designed the gate thickness equivalent to of that of the molded piece thickness. The gate width is times the thickness and the gate land length about 2mm is applicable. The pressure loss of the rectangular cross section at the gate can be calculated by the following equation. pressure loss at the gate olume flow of the resin A s f o r t h e p i n g a t e s h a p e, i t i s i m p o r t a n t t o d e t e r m i n e t h e m o s t s u i t a b l e d i a m e t e r o f t h e g a t e b y c o n s i d e r i n g f r o m t h e v i e w p o i n t o f c r a c k a n d d e f o r m a t i o n o f t h e p r o d u c t a t t h e t i m e o f c u t t i n g a n d g a t e b r e a k a g e f o r t h e m a x i m u m d i m e n s i o n, w h i l e t a k i n g d e f e c t i v e p r o b l e m s s u c h a s j e t t i n g a n d u n f i l l i n g f o r t h e m i n i m u m d i m e n s i o n i n t o c o n s i d e r a t i o n. T h e t y p i c a l p i n p o i n t g a t e s h a p e i s s h o w n i n F i g Also, Fig shows the relationship between the pin gate diameter and the thickness of the base based on the market results It is recommended to design in reference to Fig Generally, the average value of the pin gate diameter ranges from 1.0 to 2.0mm.
35 a) Thin-walled small articles b) Relatively large particles max. 1 min max. 4 Fig Shape and dimension of pinpoint gate base thickness (mm) Fig Actual relationship between the pin gate diameter and the thickness of the base The pressure loss at the gate of the circular section can be calculated by the following equation. pressure loss of the gate u viscosity of the resin q volume flow of the resin R gate radius l gate land length Gate diameter mm Notes and the design standards of the shape of the direct sprue gate are similar to the items described at the section of sprue. Fig shows the examples of standard direct blue gate.
36 Bad Fig Examples of direct sprue design It is good to determine the gate diameter of the submarine gate in a similar way of the pin gate. The standard shape of the submarine gate is shown in Fig Good Fig Example of submarine gate design The tab gate is effective for reduction of defects such as flow marks etc. but the pressure loss increases. Since this type of gate has both merits and demerits, it is recommended to use it properly. 4 P o s i t i o n o f G a t e The standards to determine the position and the number of gates are as follows. (1) Consider the thickness of the molded piece and the flowability of the resin (l/t). (2) Arrange to allow the resin flow from the thick inside of the molded piece toward the thin inside. The flowability data (bar-flow flow length) of Iupilon standard grade are shown in Fig.
37 flow length resin temperature Fig Bar-flow flow length vs resin temperature flow length resin temperature Fig Bar-flow flow length vs resin temperature
38 5 T a p e r Because the mold shrinkage percentage of Iupilon is small and its adhesion with the metal is good, a proper taper should be provided. Generally, the taper standard is in the range of 6 C o r n e r R When the corner R is small, the crack occurs due to the concentration of stress and residue stress becomes large to cause defects such as flow marks etc. It is necessary to provide the range of 0.5~1.0mmR or more for the corner. 7 M o l d M a t e r i a l The mold steel materials include carbon steel, prehardened steel, hardened steel etc. as shown in Table Especially, there is no restriction of the mold material and the material is used according to the purpose. For example, as for the mold to use the material containing glass fiber for molding, hardening steel such as SKD 61 SKS 3 etc. is used for abrasion resistance.
39 Table Mold steel material Pre har de ne d ste el
40 8 Mold heating and cooling The design of heating and cooling of the mold is important in the molding of Iupilon / NOVAREX. In the case of Iupilon / NOVAREX, it is preferable to set the mold temperature to 80 or more in order to reduce the molding strain, to improve the good appearance and the dimensional accuracy. The method of circulating oil or pressurized water for heating and cooling is the most suitable. When the core is heated locally, the method of using the chiller for cooling or thermo pipe for a core pin is recommended. Since the space heater and cartridge heater are effective in the heating but ineffective in the cooling, it is preferable to use an auxiliary heat source of heating. 9 E j e c t i o n m e t h o d It is necessary to pay attention to the ejection method because the mold release resistance from the cavity is big in the case of Iupilon / NOVAREX. When the ejection method is not suitable, defects such as cracks, deformation of the molded piece occur. Generally, the circular pin and angular pin are good for the direct ejection, the stripper plate and sleeve ejection methods are suitable for a deep product. 10 A i r v e n t When gas accumulates in the rib, the blind boss and the last filling part at the time of molding, defects such as resin burning, mold corrosion etc. due to the unfilling and the adiabatic compression occur. Especially, such a defect easily occurs when filling at high speed. Therefore, the air vent should be provided at these places. Especially, it is necessary to install air vent enough when molding the material such as compound reinforced grade with a lot of gas generation. It is good to design the air vent clearance in the range of m m. A n example of the air vent design was shown in Fig
41 Cavity ditch 1~3mm (around cavity) Water Porous metal Vent part (0.01~0.03mm) decided by resin Land Butt face (Approximately 2mm) a.dimension of vent ditch Flow of melt resin Gas flow Flow of water and gas to the outside by vacuum b. Waterline bending by using the porous metal Apart of the pin surface is connected to make the flow resistance of gas small Stagnant gas c. Waterline bending by using the fit clearance of the divided bush d. Degassing also serves as pushing pin e.degassing by bush To outside Fig Examples of air vent design
42 4 M o ld shrinkage and dimensional accuracy Mold shrinkage of Iupilon / NOVAREX varies depending on grade, molding conditions and shapes of molded piece as shown in Table Mold shrinkage percentage of various grades of Iupilon / NOVAREX varies in the range of Mold shrinkage after molding is stable for hours as shown in Table 4 3. As for the mold shrinkage anisotropy of the general grade, it is constant without depending on the flow direction of the resin and the right angle direction with it and has little anisotropy as shown in Table As for the glass fiber reinforced grade, a big difference in the mold shrinkage percentage in the flow direction of the resin and the right angle direction with it is recognized and the anisotropy is also observed. The relationship between the holding pressure and mold shrinkage percentage at the time of molding is shown in Fig. mold shrinkage percentage becomes low when increasing the holding pressure. Dimensional accuracy is affected by the material, the molded piece shape, the design and the fabrication precision of the mold, and the molding conditions. The dimensional tolerance of Polycarbonate which is published in SPI is shown in Table 4-5. The example of the unevenness and the dimension tolerance of the molded piece with the shape are shown in Table The following can be said from these results. (1)The dimensional accuracy becomes low when the shape error is included. (2)The dimension not decided by the mold, for example, the accuracy of the height dimension is low. (3)The accuracy of the material containing the glass fiber is lower than that of the unreinforced material.
43 Material Design Melt viscosity Table 4 1 Behaviour of mold shrinkage Items Combination of filling agent and mold shrinkage percentage Anisotropy of mold shrinkage percentage Thickness Gate Comments The holding pressure works well for the material with lower viscosity, the mold shrinkage percentage becomes low. When combining the filling agent, the mold shrinkage percentage becomes low. When combining the fibrous filling agent, the anisotropy occurs. As for the direction that the fiber oriented, the mold shrinkage percentage becomes low. Because the pressure loss at the side where wall thickness is thin, the mold shrinkage percentage becomes high. The mold shrinkage percentage becomes high at the side where wall thickness is thick due to slow cooling effect. There is the intermediate thickness that the mold shrinkage percentage becomes minimized When the gate diameter is large, the mold shrinkage percentage becomes low. As for the material that there is anisotropy in the mold shrinkage percentage, the mold shrinkage percentage depends on the gate position and the number. Shape Holding pressure Molding conditions The shape accuracy depends on the shape of the molded piece (roundness, cylindrical, straightness etc.) When the holding pressure is high, the mold shrinkage percentage becomes low. When the resin temperature is high, the mold shrinkage percentage becomes low. Table 4 2 Mold shrinkage percentage of various grades of Iupilon / NOVAREX Mold shrinkage percentage